1 Types of Strain l a g Engineering Strain: l o l o l b e = l l o l o (a) (b) (c) Shear Strain: FIGURE 2.1 Types of strain. (a) Tensile. (b) Compressive. (c) Shear. All deformation processes in manufacturing involve strains of these types. Tensile strains are involved in stretching sheet metal to make car bodies, compressive strains in forging metals to make turbine disks, and shear strains in making holes by punching. γ = a b
2 Tensile-Test Elastic Stress Plastic Y UTS Y Fracture Offset l o tan -1 E e o e u e f Strain (for l o = 1) l A o l e Original gage length, l o Fracture (a) l f Uniform elongation l u Neck Total elongation l f A f (b) Post-uniform elongation FIGURE 2.2 (a) Original and final shape of a standard tensile-test specimen. (b) Outline of a tensile-test sequence showing different stages in the elongation of the specimen.
3 Mechanical Properties Elongation Poisson s E (GPa) Y (MPa) UTS (MPa) in 5 mm (%) Ratio (ν) METALS (WROUGHT) Aluminum and its alloys Copper and its alloys Lead and its alloys Magnesium and its alloys Molybdenum and its alloys Nickel and its alloys Steels Stainless steels Titanium and its alloys Tungsten and its alloys NONMETALLIC MATERIALS Ceramics Diamond Glass and porcelain Rubbers Thermoplastics Thermoplastics, reinforced Thermosets Boron fibers Carbon fibers Glass fibers (S, E) Kevlar fibers (29, 49, 129) Spectra fibers (9, 1) Note: In the upper table, the lowest values for E, Y, and UTS and the highest values for elongation are for the pure metals. Multiply GPa by 145, to obtain psi, and MPa by 145 to obtain psi. For example 1 GPa = 14,5 ksi, and 1 MPa = 14,5 psi. TABLE 2.1 Typical mechanical properties of various materials at room temperature. See also Tables 1.1, 1.4, 1.8, 11.3 and 11.7.
4 Loading & Unloading; Elongation mm High-purity aluminum-annealed 6 Stress Unload Load Elastic recovery Permanent deformation Strain FIGURE 2.3 Schematic illustration of loading and unloading of a tensile-test specimen. Note that during unloading the curve follows a path parallel to the original elastic slope. Elongation (%) Brass Monel 11-O Aluminum Mild steel Structural silicon steel Magnesium Copper Gage length (in.) FIGURE 2.4 Total elongation in a tensile test as a function of original gage length for various metals. Because necking is a local phenomenon, elongation decreases with gage length. Standard gage length is usually 2 in. (5 mm), although shorter ones can be used if larger specimens are not available.
5 True Stress and True Strain True stress σ = P A True strain ( ) l ε = ln l o = ln ( Ao A ) = ln ( Do D ) 2 = 2ln ( Do D ) TABLE 2.2 Comparison of engineering and true strains in tension e ɛ
6 True Stress - True Strain Curve Fracture True stress K Y f Y = K n Log n 1 1 f True strain ( ) True stress (psi x 1 3 ) 1 1 Y (a) (c) K = 25, Log (b) n = True strain ( ) 1 n FIGURE 2.5 (a) True stress--true strain curve in tension. Note that, unlike in an engineering stress-strain curve, the slope is always positive and that the slope decreases with increasing strain. Although in the elastic range stress and strain are proportional, the total curve can be approximated by the power expression shown. On this curve, Y is the yield stress and Yf is the flow stress. (b) True stresstrue strain curve plotted on a log-log scale. (c) True stress-true strain curve in tension for 11-O aluminum plotted on a log-log scale. Note the large difference in the slopes in the elastic and plastic ranges. Source: After R. M. Caddell and R. Sowerby.
7 Power Law Flow Rule Material K (MPa) n Aluminum, 11-O T O O T O 4.17 Brass, 73, annealed , cold rolled Bronze (phosphor), annealed Cobalt-base alloy, heat treated 27.5 Copper, annealed Molybdenum, annealed Steel, low carbon, annealed hot rolled annealed cold rolled annealed cold rolled annealed P-H, annealed , annealed stainless, annealed stainless, annealed 96.1 Note: 1 MPa = 14,5 psi. Flow rule: σ = Kε n K = Strength coefficient n = Strain hardening exponent TABLE 2.3 Typical values for K and n in Eq at room temperature.
8 True Stress-True Strain for Various Materials Stainless steel 12 True stress (psi x 1 3 ) Brass, as received 865 Steel Brass, annealed 1112 CR Steel 12 Steel Steel 8 Copper, annealed 224-T36 Al O Al O Al 11-O Al H14 Al True strain ( ) MPa FIGURE 2.6 True stress-true strain curves in tension at room temperature for various metals. The point of intersection of each curve at the ordinate is the yield stress Y; thus, the elastic portions of the curves are not indicated. When the K and n values are determined from these curves, they may not agree with those given in Table 2.3 because of the different sources from which they were collected. Source: S. Kalpakjian.
9 Idealized Stress-Strain Curves Stress tan -1 E = EP Y = Y Y = E = Y Strain (a) (b) Y/E (c) Y =Y + E p! tan -1 E p Y E Y + E p ( -Y/E ) True stress K = K n n = 1 < n < 1 n = (d) Y/E (e) 1 True strain (P) FIGURE 2.7 Schematic illustration of various types of idealized stressstrain curves. (a) Perfectly elastic. (b) Rigid, perfectly plastic. (c) Elastic, perfectly plastic. (d) Rigid, linearly strain hardening. (e) Elastic, linearly strain hardening. The broken lines and arrows indicate unloading and reloading during the test. FIGURE 2.8 The effect of strain-hardening exponent n on the shape of true stresstrue strain curves. When n = 1, the material is elastic, and when n =, it is rigid and perfectly plastic.
10 Temperature and Strain Rate Effects Stress (MPa) Stress (psi ) ( C) Elastic modulus Tensile strength Yield strength Elongation Elastic modulus (GPa) Elongation (%) Tensile strength (psi x 1 3 ) C MPa Temperature ( F) Strain rate (s -1 ) FIGURE 2.9 Effect of temperature on mechanical properties of a carbon steel. Most materials display similar temperature sensitivity for elastic modulus, yield strength, ultimate strength, and ductility. FIGURE 2.1 The effect of strain rate on the ultimate tensile strength of aluminum. Note that as temperature increases, the slope increases. Thus, tensile strength becomes more and more sensitive to strain rate as temperature increases. Source: After J. H. Hollomon.
11 Typical Strain Rates in Metalworking Process True Strain Deformation Speed (m/s) Strain Rate (s 1 ) Cold Working Forging, rolling Wire and tube drawing Explosive forming Hot working and warm working Forging, rolling Extrusion Machining Sheet-metal forming Superplastic forming TABLE 2.4 Typical ranges of strain, deformation speed, and strain rates in metalworking processes.
12 Effect on Homologous Temperature.25 Strain rate sensitivity exponent (m) Copper Steel Aluminum 34 Stainless Titanium Rene 41 Mo-T2C Homologous temperature, T T m FIGURE 2.11 Dependence of the strainrate sensitivity exponent m on the homologous temperature T/Tm for various materials. T is the testing temperature and Tm is the melting point of the metal, both on the absolute scale. The transition in the slopes of the curve occurs at about the recrystallization temperature of the metals. Source: After F. W. Boulger.
13 Strain Rate Effects C Material Temperature, C psi 1 3 MPa m Aluminum Aluminum alloys Copper Copper alloys (brasses) Lead Magnesium Steel Low carbon Medium carbon Stainless Titanium Titanium alloys Ti-6Al-4V Zirconium at a strain rate of s 1. Note: As temperature increases, C decreases and m increases. As strain increases, C increases and m may increase or decrease, or it may become negative within certain ranges of temperature and strain. Source: After T. Altan and F.W. Boulger. σ = C ε m C = Strength coefficient m = Strain-rate sensitivity exponent TABLE 2.5 Approximate range of values for C and m in Eq. (2.16) for various annealed metals at true strains ranging from.2 to 1..
14 Effect of Strain Rate Sensitivity on Elongation Total elongation (%) Ti 5A1 2.5Sn Ti 6A1 4V Zircaloy 4 High- and ultra-highcarbon steels Post-uniform elongation (%) A-K Steel HSLA Steel C.R. Aluminum (11) 236-T4 Aluminum 33-O Aluminum 5182-O Aluminum 5182-O Al (15C) 7-3 Brass Zn-Ti Alloy m (a) FIGURE 2.12 (a) The effect of strain-rate sensitivity exponent m on the total elongation for various metals. Note that elongation at high values of m approaches 1%. Source: After D. Lee and W.A. Backofen. (b) The effect of strain-rate sensitivity exponent m on the post uniform (after necking) elongation for various metals. Source: After A.K. Ghosh..2 m (b).4.6
15 Hydrostatic Pressure & Barreling 5 MPa Copper True strain at fracture ( f ) Zinc Magnesium Aluminum Cast iron Hydrostatic pressure (ksi) FIGURE 2.13 The effect of hydrostatic pressure on true strain at fracture in tension for various metals. Even cast iron becomes ductile under high pressure. Source: After H.L.D. Pugh and D. Green. FIGURE 2.14 Barreling in compressing a round solid cylindrical specimen (775-O aluminum) between flat dies. Barreling is caused by friction at the die-specimen interfaces, which retards the free flow of the material. See also Figs.6.1 and 6.2. Source: K.M. Kulkarni and S. Kalpakjian.
16 Plane-Strain Compression Test w > 5h w > 5b b > 2h to 4h h b w Yield stress in plane strain: Y = 2 3 Y = 1.15Y FIGURE 2.15 Schematic illustration of the plane-strain compression test. The dimensional relationships shown should be satisfied for this test to be useful and reproducible. This test gives the yield stress of the material in plane strain, Y. Source: After A. Nadai and H. Ford.
17 Tension & Compression; Baushinger Effect 16 Tension True stress (ksi) Tension Compression 1 5 MPa Y 2Y P True strain ( ) FIGURE 2.16 True stress-true strain curve in tension and compression for aluminum. For ductile metals, the curves for tension and compression are identical. Source: After A.H. Cottrell. Compression FIGURE 2.17 Schematic illustration of the Bauschinger effect. Arrows show loading and unloading paths. Note the decrease in the yield stress in compression after the specimen has been subjected to tension. The same result is obtained if compression is applied first, followed by tension, whereby the yield stress in tension decreases.
18 Disk & Torsion Tests P l r r r t Fracture P σ = 2P πdt FIGURE 2.18 Disk test on a brittle material, showing the direction of loading and the fracture path. This test is useful for brittle materials, such as ceramics and carbides. τ = T 2πr 2 t l FIGURE 2.19 A typical torsion-test specimen. It is mounted between the two heads of a machine and is twisted. Note the shear deformation of an element in the reduced section. r γ = rφ l
19 Simple vs. Pure Shear = (a) (b) FIGURE 2.2 Comparison of (a) simple shear and (b) pure shear. Note that simple shear is equivalent to pure shear plus a rotation.
20 Three- and Four-Point Bend-Tests Maximum bending moment σ = Mc I (a) (b) FIGURE 2.21 Two bend-test methods for brittle materials: (a) threepoint bending; (b) four-point bending. The shaded areas on the beams represent the bending-moment diagrams, described in texts on the mechanics of solids. Note the region of constant maximum bending moment in (b), whereas the maximum bending moment occurs only at the center of the specimen in (a).
21 Hardness Tests Shape of indentation Test Indenter Side view Top view Load, P Hardness number Brinell 1-mm steel or tungsten carbide ball D d d 5 kg 15 kg 3 kg 2P HB = ( D)(D - D 2 - d 2 ) Vickers Diamond pyramid 136 L 1 12 kg HV = 1.854P L 2 b Knoop Diamond pyramid L/b = 7.11 b/t = 4. t L 25 g 5 kg HK = 14.2P L 2 Rockwell A C D B F G E Diamond cone 1 - in. diameter 16 steel ball 1 - in. diameter 8 steel ball 12 t = mm t = mm 6 kg 15 kg 1 kg 1 kg 6 kg 15 kg 1 kg HRA HRC HRD HRB HRF HRG HRE = 1-5t = 13-5t FIGURE 2.22 General characteristics of hardness testing methods. The Knoop test is known as a microhardness test because of the light load and small impressions. Source: After H.W. Hayden, W.G. Moffatt, and V. Wulff.
22 d Hardness Test Considerations d (a) FIGURE 2.23 Indentation geometry for Brinell hardness testing: (a) annealed metal; (b) workhardened metal. Note the difference in metal flow at the periphery of the impressions. (b) Hardness (psi x 1 3 ) MPa Carbon steels, annealed Aluminum, cold worked Carbon steels, cold worked Brinell hardness (kg/mm 2 ) FIGURE 2.25 Bulk deformation in mild steel under a spherical indenter. Note that the depth of the deformed zone is about one order of magnitude larger than the depth of indentation. For a hardness test to be valid, the material should be allowed to fully develop this zone. This is why thinner specimens require smaller indentations. Source: Courtesy of M.C. Shaw and C.T. Yang Yield stress (psi x 1 3 ) FIGURE 2.24 Relation between Brinell hardness and yield stress for aluminum and steels. For comparison, the Brinell hardness (which is always measured in kg/mm 2 ) is converted to psi units on the left scale.
23 Fatigue Stress amplitude, S (MPa) Steel 214-T6 Aluminum alloy Endurance limit psi x Number of cycles, N Number of cycles, N Stress amplitude, S (MPa) Epoxy PTFE (a) (b) Phenolic Diallyl-phthalate Polycarbonate Polysulfone Nylon (dry) psi x 1 3 FIGURE 2.26 Typical S-N curves for two metals. Note that, unlike steel, aluminum does not have an endurance limit..8 MPa FIGURE 2.27 Ratio of fatigue strength to tensile strength for various metals, as a function of tensile strength. Endurance limit/tensile strength Titanium Steels Cast irons Copper alloys.3.2 Cast Aluminum alloys magnesium.1 alloys Wrought magnesium alloys Tensile strength (psi x 1 3 )
24 Creep & Impact Rupture Pendulum Strain Primary Secondary Tertiary Pendulum Specimen (1 x 1 x 55 mm) Specimen (1 x 1 x 75 mm) Notch Instantaneous deformation (a) (b) Time FIGURE 2.28 Schematic illustration of a typical creep curve. The linear segment of the curve (constant slope) is useful in designing components for a specific creep life. FIGURE 2.29 Impact test specimens: (a) Charpy; (b) lzod.
25 Residual Stresses Tensile a b c o Compressive (a) (c) o a d (b) f (d) e FIGURE 2.3 Residual stresses developed in bending a beam made of an elastic, strain-hardening material. Note that unloading is equivalent to applying an equal and opposite moment to the part, as shown in (b). Because of nonuniform deformation, most parts made by plastic deformation processes contain residual stresses. Note that the forces and moments due to residual stresses must be internally balanced.
26 Distortion due to Residual Stress Before After Before After (a) (b) Before After (c) FIGURE 2.31 Distortion of parts with residual stresses after cutting or slitting: (a) rolled sheet or plate; (b) drawn rod; (c) thin-walled tubing. Because of the presence of residual stresses on the surfaces of parts, a round drill may produce an oval-shaped hole because of relaxation of stresses when a portion is removed.
27 Elimination of Residual Stresses Tension Stress Compressive Tensile t c Y c Y t 2Y! c! t Compression (a) (b) (c) (d) FIGURE 2.32 Elimination of residual stresses by stretching. Residual stresses can be also reduced or eliminated by thermal treatments, such as stress relieving or annealing.
28 State of Stress in Metalworking! 1! 1 (a)! 2! 1! 1 (b)! 2! 1! 1! 2! 2 FIGURE 2.33 The state of stress in various metalworking operations. (a) Expansion of a thin-walled spherical shell under internal pressure. (b) Drawing of round rod or wire through a conical die to reduce its diameter; see Section 6.5 (c) Deep drawing of sheet metal with a punch and die to make a cup; see Section 7.6. (c)
29 Strain State in Necking R Correction factor due to Bridgman: Distribution of axial stress a Maximum axial stress Average axial true stress σ σ av = ( 1 + 2R a 1 ) [( 1 + a )] 2R Distribution of radial or tangential stress = True stress in uniaxial tension FIGURE 2.34 Stress distribution in the necked region of a tension-test specimen.
30 States of Stress! 1! 1! 1! 1! 2! 1 (a) (c) (e)! 1! 1! 2 p p (b)! 1 (d) p p (f) p p FIGURE 2.35 Examples of states of stress: (a) plane stress in sheet stretching; there are no stresses acting on the surfaces of the sheet. (b) plane stress in compression; there are no stresses acting on the sides of the specimen being compressed. (c) plane strain in tension; the width of the sheet remains constant while being stretched. (d) plane strain in compression (see also Fig. 2.15); the width of the specimen remains constant due to the restraint by the groove. (e) Triaxial tensile stresses acting on an element. (f) Hydrostatic compression of an element. Note also that an element on the cylindrical portion of a thin-walled tube in torsion is in the condition of both plane stress and plane strain (see also Section ).
31 Yield Criteria Compression Tension!! 1! 1 1!1 Y Maximum-shear Y stress criterion! 1 Tension Distortion-energy criterion Maximum-shear-stress criterion: σ max σ min = Y Distortion-energy criterion:! 1!! 1 Compression 1! 1 (σ 1 σ 2 ) 2 + (σ 2 σ 3 ) 2 + (σ 3 σ 1 ) 2 = 2Y 2 FIGURE 2.36 Plane-stress diagrams for maximum -shear-stress and distortion-energy criteria. Note that 2 =.
32 Flow Stress and Work of Deformation True stress Y f Y Y u 1 Flow stress: Ȳ = Kεn 1 n + 1 True strain (!) FIGURE 2.37 Schematic illustration of true stress-true strain curve showing yield stress Y, average flow stress, specific energy u1 and flow stress Yf.! 1 Specific energy u = Z ε σd ε
33 Ideal & Redundant Work (a) Total specific energy: u total = u ideal + u f riction + u redundant (b) (c) FIGURE 2.38 Deformation of grid patterns in a workpiece: (a) original pattern; (b) after ideal deformation; (c) after inhomogeneous deformation, requiring redundant work of deformation. Note that (c) is basically (b) with additional shearing, especially at the outer layers. Thus (c) requires greater work of deformation than (b). See also Figs. 6.3 and Efficiency: η = u ideal u total
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B-306) INTRODUCTION TENSION TEST Mechanical testing
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
Hardness Test Chapter 9 Subjects of interest Introduction/objectives Brinell hardness Meyer hardness Vickers hardness Rockwell hardness Microhardness tests Relationship between hardness and the flow curve
1 Unit 6: EXTRUSION Introduction: Extrusion is a metal working process in which cross section of metal is reduced by forcing the metal through a die orifice under high pressure. It is used to produce cylindrical
Laboratory 2 Hardness Testing Objectives Students are required to understand the principles of hardness testing, i.e., Rockwell, Brinell and Vickers hardness tests. Students are able to explain variations
5. MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS Samples of engineering materials are subjected to a wide variety of mechanical tests to measure their strength, elastic constants, and other material
Example: 1 A 300-mm-wide strip 25 mm thick is fed through a rolling mill with two powered rolls each of radius = 250 mm. The work thickness is to be reduced to 22 mm in one pass at a roll speed of 50 rev/min.
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, Jan-Feb 2016, pp. 119-130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
Lecture slides on rolling By: Dr H N Dhakal Lecturer in Mechanical and Marine Engineering, School of Engineering, University of Plymouth Bulk deformation forming (rolling) Rolling is the process of reducing
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 2322-5009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277-284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
Sheet metal operations - Bending and related processes R. Chandramouli Associate Dean-Research SASTRA University, Thanjavur-613 401 Table of Contents 1.Quiz-Key... Error! Bookmark not defined. 1.Bending
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE Ali Fatemi-University of Toledo All Rights Reserved Chapter 8 Residual Stresses & Their Effects 1 RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE
STRESS-STRAIN CURVES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 August 23, 2001 Introduction Stress-strain curves are an extremely
Homework solutions for test 2 HW for Lecture 7 22.2 What is meant by the term faying surface? Answer. The faying surfaces are the contacting surfaces in a welded joint. 22.3 Define the term fusion weld.
NOTCHES AND THEIR EFFECTS Ali Fatemi - University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations S-N Approach for Notched Members
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
ME 354, MECHANICS OF MATERIALS LABORATORY 01 Januarly 2000 / mgj MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS: HARDNESS TESTING* PURPOSE The purpose of this exercise is to obtain a number of experimental
MME131: Lecture 15 Mechanical properties 3 Bend test and hardness test of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Bend test of brittle materials Hardness testing
T dition CHTR MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University Stress and Strain xial oading - Contents Stress & Strain: xial oading
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0 - INTRODUCTION See General Lab Report Format
Technical Data BLUE SHEET Allegheny Ludlum Corporation Pittsburgh, PA Martensitic Stainless Steels Types 410, 420, 425 Mod, and 440A GENERAL PROPERTIES Allegheny Ludlum Types 410, 420, 425 Modified, and
Typical stress-strain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A = --- A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
METALLURGY AND FOUNDRY ENGINEERING Vol. 33, 2007, No. 1 Jerzy Kajtoch * STRAIN IN THE UPSETTING PROCESS 1. INTRODUCTION Upsetting is an technological operation of open die forging, which is performed in
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
Mechanical Properties and Fracture Analysis of Glass David Dutt Chromaglass, Inc. IES ALC Williamsburg 2006 2 IES ALC Williamsburg 2006 3 Outline The Ideal The Practical The Reality IES ALC Williamsburg
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
1 Introduction to Hardness Testing Hardness has a variety of meanings. To the metals industry, it may be thought of as resistance to permanent deformation. To the metallurgist, it means resistance to penetration.
CHAPTER1 Fundamentals of Extrusion The first chapter of this book discusses the fundamentals of extrusion technology, including extrusion principles, processes, mechanics, and variables and their effects
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
Superior performance Co-Ni Alloy Product (SPRON) Product Catalogue 21 211 Superior performance Co-Ni Alloy Product (SPRON) solves designers problems " " is a special metal (Co-Ni alloy) developed for mechanical
Designation: E 40 02 Standard Conversion Tables for Metals Relationship Among Brinell,, Rockwell, Superficial, Knoop, and Scleroscope This standard is issued under the fixed designation E 40; the number
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
PAGE 1/10 1 Density The density of optical glass varies from 239 for N-BK10 to 603 for SF66 In most cases glasses with higher densities also have higher refractive indices (eg SF type glasses) The density
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1 - LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
ITU Department of Mechanical Engineering MANUFACTURING PROPERTIES of ENGINEERING MATERIALS Lecture Notes Prof.Dr.Ahmet Aran 2007 CONTENTS 1. Engineering Materials and Their Properties 1.1. Classification
Stress-Life Diagram (S-N Diagram) The basis of the Stress-Life method is the Wohler S-N diagram, shown schematically for two materials in Figure 1. The S-N diagram plots nominal stress amplitude S versus
HAPTER Reinforced oncrete Design Fifth Edition MATERIALS AND MEHANIS OF BENDING A. J. lark School of Engineering Department of ivil and Environmental Engineering Part I oncrete Design and Analysis b FALL
North American Stainless Flat Products Stainless Steel Sheet T409 INTRODUCTION NAS 409 is an 11% chromium, stabilized ferritic stainless steel. It is not as resistant to corrosion or high-temperature oxidation
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
ALLOY 2205 DATA SHEET UNS S32205, EN 1.4462 / UNS S31803 GENERAL PROPERTIES ////////////////////////////////////////////////////// //// 2205 (UNS designations S32205 / S31803) is a 22 % chromium, 3 % molybdenum,
ALLOY 625 DATA SHEET //// Alloy 625 (UNS designation N06625) is a nickel-chromium-molybdenum alloy possessing excellent resistance to oxidation and corrosion over a broad range of corrosive conditions,
HAYNES 25 alloy Principle Features Excellent High-Temperature Strength and Good Oxidation Resistance HAYNES 25 alloy (UNS R30605) is a cobalt-nickel- chromium-tungsten alloy that combines excellent high-temperature
Hardened Concrete Lecture No. 14 Strength of Concrete Strength of concrete is commonly considered its most valuable property, although in many practical cases, other characteristics, such as durability
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: email@example.com Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In this section work hardening models that are applicable to different
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
T O O L S T E E L F A C T S RAMAX S Prehardened stainless holder steel Wherever tools are made Wherever tools are used This information is based on our present state of knowledge and is intended to provide
Application of Web-Based Bar Fatigue Database Database Development Thomas G. Oakwood Bar Steel Fatigue Database- Objectives Develop a strain-controlled fatigue database for carbon and low alloy bar steels
Hardness Testing at Elevated Temperatures SJ Shaffer, Ph.D. Bruker-TMT Steven.firstname.lastname@example.org Outline What is Hardness? How is Hardness Measured? Overview of Hardness Test Methods Hardness Testing
IMPACT TESTING Objective To conduct Charpy V-notch impact test and determine the ductile-brittle transition temperature of steels. Equipment Coolants Standard Charpy V-Notched Test specimens Impact tester
Mechanical Metallurgy Lecturer Assessment Dr. Assignment 20 (homework, quiz, attendance) Midterm exam 40 Final exam 40 Total 100 Mechanical Metallurgy Subject of interests Part I Mechanical fundamentals
TITANIUM FABRICATION CORP. Titanium, Zirconium, and Tantalum Clad Construction General Considerations In many applications, particularly for large pressure vessels designed for high temperature and pressure,
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
Chapter 5 Bridge Deck Slabs Bridge Engineering 1 Basic types of bridge decks In-situ reinforced concrete deck- (most common type) Pre-cast concrete deck (minimize the use of local labor) Open steel grid
Carbon Fiber Reinforced Polymer (CFRP) Tape is used for structural strengthening of concrete, masonry or timber elements using the technique known as Near Surface Mount or NSM strengthening. Use of CFRP
Chapter 2 PROPERTIES, IDENTIFICATION, AND HEAT TREATMENT OF METALS GENERAL PURPOSE This chapter contains basic information pertaining to properties and identification of metal and heat-treating procedures
Chapter 17: Springs It must be confessed that the inventors of the mechanical arts have been much more useful to men than the inventors of syllogisms. Voltaire A collection of helical compression springs.
Mechanical Properties - Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
National Aeronautics and Space Administration Lyndon B. Johnson Space Center Houston, Texas 77058 REVISION A JULY 6, 1998 REPLACES BASELINE SPACE SHUTTLE CRITERIA FOR PRELOADED BOLTS CONTENTS 1.0 INTRODUCTION..............................................
4.461: Building Technology 1 CONSTRUCTION AND MATERIALS Professor John E. Fernandez FALL TERM 2004 SCHOOL OF ARCHITECTURE AND PLANNING: MIT Concrete and Composites Stadelhofen Station Zurich Santiago Calatrava
UDDEHOLM VANADIS 30 SUPERCLEAN UDDEHOLMS AB No part of this publication may be reproduced or transmitted for commercial purposes without permission of the copyright holder. This information is based on
AN EXPLANATION OF JOINT DIAGRAMS When bolted joints are subjected to external tensile loads, what forces and elastic deformation really exist? The majority of engineers in both the fastener manufacturing
2.6.4 Simulation of Residual Stresses in an Induction Hardened Roll Ludwig Hellenthal, Clemens Groth Walzen Irle GmbH, Netphen-Deuz, Germany CADFEM GmbH, Burgdorf/Hannover, Germany Summary A heat treatment
North American Stainless Flat Products Stainless Steel Grade Sheet 430 (S43000)/ EN 1.4016 Introduction: SS430 is a low-carbon plain chromium, ferritic stainless steel without any stabilization of carbon
THYROPLAST 3 / 3 SUPRA C Cr. 13. Corrosion-resistant, good polishability. We recommend the use of THYROPLAST 3 SUPRA (ESR) for the highest demands on polishability. Coefficient of thermal expansion 1 -
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
7-1 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length